# Volume Holograms in Photopolymers: Comparison between Analytical and Rigorous Theories

^{1}

^{2}

^{3}

^{*}

## Abstract

**:**

## 1. Introduction

## 2. Theoretical Background

**K**is the wave vector and can be expressed as function of the grating period; Λ, or as function of the frequency, f:

_{1}is the refractive index modulation; λ

_{0}is the wavelength in vacuum; and ϑ is a parameter that measures the Bragg angle deviation.

**ρ**

_{i}=

**ρ**

_{0}+i

**K**i = 0, ±1, ±2,...

_{i}are the called obliquity factors and are the cosine of the angles that the propagation vectors of the different orders form with the z-axis. In the particular case of non-slanted diffraction gratings, C

_{i}= cosθ

_{0}, where θ

_{0}is the angle of reconstruction inside the medium.

_{1}<< n

_{0}. The cases analyze in this work are consistent with condition.

## 3. Gratings Recorded in Photopolymers

#### 3.1. Theoretical Simulations

_{1}= 0.004 was used [36]. In the second place we performed the analysis with a value of the refractive index modulation n

_{1}= 0.011, a value which is near of maximum for materials based in PVA/AA and is achieved using a crosslinker monomer, NN’,methylene-bis-acrylamide (BMA) [35,36].

_{1}= 0.004, at first Bragg’s condition (Ω takes the value 8.3). The value of Ω shows that we are in Bragg’s regime, and as can be expected the predictions of the three theories are similar (Kogelnik, CW and RCW) in the range of thickness studied.

**Table 1.**Values of the parameters of the phase transmission gratings for different spatial frequencies.

Refractive index modulation | f = 350 lines/mm | f = 500 lines/mm | f = 750 lines/mm |
---|---|---|---|

n_{1} = 0.004 | Ω ~ 8 | Ω ~ 17 | Ω ~ 38 |

n_{1} = 0.011 | Ω ~ 3 | Ω ~ 6 | Ω ~ 14 |

**Figure 1.**Diffraction efficiency of order +1 (first order diffracted), at first Bragg’s angle. The spatial frequency is 350 lines/mm and the refractive index modulation is n

_{1}= 0.004.

**Figure 2.**Efficiency of order 0 (zero order diffracted), at first Bragg’s angle. The spatial frequency is 350 lines/mm and the refractive index modulation is n

_{1}= 0.004.

_{1}= 0.011) for the same spatial frequency the curves presented in Figure 3 and Figure 4 can be obtained (first and zero orders versus thickness at first Bragg angle condition), Ω takes a value of 3, so this grating cannot be classified as a volume one. If these figures are analyzed we can see that there exist deviations between the predictions using Kogelnik’s theory and the results obtained using CW and RCW. This fact occurs because the secondary orders cannot be neglected and part of the energy is diffracted in other directions (secondary diffracted orders). It is also interesting to remark that in all the cases the predictions of CW and RCW are very similar, what shows that the second derivates can be neglected in Equation (8). The results obtained by these two theories are also similar for secondary orders. The energy of orders −1 and +2 as a function of the thickness of the grating are represented in Figure 5.

**Figure 3.**Diffraction efficiency of order +1 (first order diffracted), at first Bragg’s angle. The spatial frequency is 350 lines/mm and the refractive index modulation is n

_{1}= 0.011.

**Figure 4.**Efficiency of order 0 (zero order diffracted), at first Bragg’s angle. The spatial frequency is 350 lines/mm and the refractive index modulation is n

_{1}= 0.011.

**Figure 5.**Efficiency of the orders −1 and +2, at first Bragg’s angle. The spatial frequency is 350 lines/mm and the refractive index modulation is n

_{1}= 0.011.

_{1}= 0.011). In these figures there is good agreement between the CW and RCW theories, but the results obtained by using Kogelnik Coupled Wave Theory slightly deviate from those of RCW and CW theories. This is due to the existence of multi-order diffraction, although the results are clearly closer than in the case of 350 lines/mm.

**Figure 6.**Diffraction efficiency of order +1 (first order diffracted), at first Bragg’s angle. The spatial frequency is 500 lines/mm and the refractive index modulation is n

_{1}= 0.011.

**Figure 7.**Efficiency of order 0 (zero order diffracted), at first Bragg’s angle. The spatial frequency is 500 lines/mm and the refractive index modulation is n

_{1}= 0.011.

_{1}= 0.011 (Ω = 14). It is evident that in this case the agreement between the three theories is almost perfect, so in this case Kogelnik’s theory is highly applicable to analyze these gratings at first Bragg’s angle.

**Figure 8.**Diffraction efficiency of order +1 (first order diffracted), at first Bragg’s angle. The spatial frequency is 750 lines/mm and the refractive index modulation is n

_{1}= 0.011.

**Figure 9.**Efficiency of order 0 (zero order diffracted), at first Bragg’s angle. The spatial frequency is 750 lines/mm and the refractive index modulation is n

_{1}= 0.011.

#### 3.2. Experimental Results

^{2}.

_{1}= 0.0102, and α = 0.0056 μm

^{−1}).

**Figure 11.**Diffraction efficiency of the order +1 for volume transmission gratings recorded in polyvinyl-alcohol/acrylamide (PVA/AA) with spatial frequency 1125 lines/mm and 23 µm of thickness.

_{1}= 0.00476, d = 69 µm and α = 0.0042 μm

^{−1}.

**Figure 12.**Diffraction efficiency of order +1 for volume transmission gratings recorded in PVA/AA with spatial frequency 545 lines/mm and 69 µm of thickness at first Bragg’s angle.

_{1}= 0.011. In Figure 13 it can be seen the discrepancies in the results provided by these two theories. Therefore the approximations made in the Kogelnik’s analysis cannot be done in this case. When Kogelnik’s theory is used to fit the angular response of gratings with spatial frequency of 350 lines/mm important errors will be made in the values of thickness and refractive modulation.

**Figure 13.**Diffraction efficiency of order +1 for volume transmission gratings with spatial frequency 350 lines/mm, n

_{1}= 0.011 and 25 µm of thickness at first Bragg’s angle.

## 4. Conclusions

## Acknowledgments

## References

- Neumann, J.; Wieking, K.S.; Kip, D. Direct laser writing of surface reliefs in dry, self-developing photopolymer films. Appl. Opt.
**1999**, 38, 5418–5421. [Google Scholar] [CrossRef] [PubMed] - Li, X.T.; Natansohn, A.; Rochon, P. Photoinduced liquid crystal alignment based on a surface relief grating in an assembled cell. Appl. Phys. Lett.
**1999**, 74, 3791–3793. [Google Scholar] [CrossRef] - Márquez, A.; Gallego, S.; Ortuño, M.; Fernández, E.; Alvarez, M.L.; Beléndez, A.; Pascual, I. Generation of diffractive optical elements onto a photopolymer using a liquid crystal display. Proc. SPIE
**2010**, 7717. Available online: http://rua.ua.es/dspace/bitstream/10045/14247/1/SPIE_vol7717_art7717-12_2010.pdf (accessed on 2 August 2012). [Google Scholar] [CrossRef] - Lechner, M.D. Photopolymers for optical memories and waveguides. Electron. Prop. Polym. Relat. Compd.
**1985**, 63, 301–308. [Google Scholar] - Coufal, H.J.; Psaltis, D.; Sincerbox, G.T. Holographic Data Storage; Springer-Verlag: Berlin, Germany, 2000. [Google Scholar]
- Márquez, A.; Neipp, C.; Beléndez, A.; Gallego, S.; Ortuño, M.; Pascual, I. Edge-enhanced imaging with polyvinyl alcohol/acrylamide photopolymer gratings. Opt. Lett.
**2003**, 28, 1510–1512. [Google Scholar] [CrossRef] [PubMed] - Manivannan, G.; Lessard, R.A. Trends in holographic recording materials. Trends Polym. Sci.
**1994**, 2, 282–290. [Google Scholar] - Curtis, K.; Dhar, L.; Murphy, L.; Hill, A. Future Developments in Holographic Data Storage: From Theory to Practical Systems; John Wiley & Sons: Chichester, UK, 2010. [Google Scholar]
- Martin, S.; Leclere, P.E.; Renotte, Y.L.; Toal, V.; Lion, Y.F. Characterization of an acrylamide-based dry photopolymer holographic recording material. Opt. Eng.
**1994**, 33, 3942–3946. [Google Scholar] [CrossRef] - Curtis, K.; Psaltis, D. Characterization of the Du-Pont photopolymer for 3-dimensional holographic storage. Appl. Opt.
**1994**, 33, 5396–5399. [Google Scholar] [CrossRef] [PubMed] - Gallego, S.; Ortuño, M.; Neipp, C.; Márquez, A.; Beléndez, A.; Pascual, I.; Kelly, J.V.; Sheridan, J.T. Physical and effective optical thickness of the holographic diffraction gratings recorded in photopolymers. Opt. Express
**2005**, 13, 3543–3557. [Google Scholar] [CrossRef] [PubMed] - Gallego, S.; Ortuño, M.; Neipp, C.; Fernández, E.; Beléndez, A.; Pascual, I. Improved maximum uniformity and capacity of multiple holograms recorded in absorbent photopolymers. Opt. Express
**2007**, 15, 9308–9319. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Martin, S.; Feely, C.A.; Toal, V. Holographic recording characteristics of an acrylamide-based photopolymer. Appl. Opt.
**1994**, 36, 5757–5768. [Google Scholar] [CrossRef] - O’Neill, F.T.; Lawrence, J.R.; Sheridan, J.T. Thickness variation of self-processing acrylamide-based photopolymer and reflection holography. Opt. Eng.
**2001**, 40, 533–539. [Google Scholar] [CrossRef] - Close, C.E.; Gleeson, M.R.; Sheridan, J.T. Monomer diffusion rates in photopolymer material: Part I: Low spatial frequency holographic gratings. J. Opt. Soc. Am. B
**2011**, 28, 658–666. [Google Scholar] [CrossRef] - Gallego, S.; Márquez, A.; Méndez, D.I.; Marini, S.; Beléndez, A.; Pascual, I. Spatial-phase-modulation-based study of polyvinyl-alcohol/acrylamide photopolymers in the low spatial frequency range. Appl. Opt.
**2009**, 48, 4403–4413. [Google Scholar] [CrossRef] [PubMed] - Naydenova, I.; Mihaylova, E.; Martin, S.; Toal, V. Holographic patterning of acrylamide-based photopolymer surface. Opt. Express
**2005**, 13, 4878–4889. [Google Scholar] [CrossRef] [PubMed] - Kogelnik, H. Coupled wave theory for thick hologram gratings. Bell Syst. Tech. J.
**1969**, 48, 2909–2947. [Google Scholar] [CrossRef] - Gallego, S.; Ortuño, M.; Neipp, C.; García, C.; Beléndez, I.; Pascual, I. Overmodulation effects in volume holograms recorded on photopolymers. Opt. Commun.
**2003**, 215, 263–269. [Google Scholar] [CrossRef] - Gallego, S.; Ortuño, M.; Neipp, C.; García, C.; Beléndez, I.; Pascual, I. Temporal evolution of the angular response of a holographic diffraction grating in PVA/acrylamide photopolymer. Opt. Express
**2003**, 11, 181–190. [Google Scholar] [CrossRef] [PubMed] - Moharam, M.G.; Gaylord, T.K. Rigorous coupled-wave analysis of planar-grating diffraction. J. Opt. Soc. Am.
**1981**, 71, 811–818. [Google Scholar] [CrossRef] - Neipp, C.; Beléndez, A.; Gallego, S.; Ortuño, M.; Pascual, I.; Sheridan, J.T. Angular responses of the first and second diffracted orders in transmission diffraction grating recorded on photopolymer material. Opt. Express
**2003**, 11, 1835–1843. [Google Scholar] [CrossRef] [PubMed] - Wu, S.; Glytsis, E.N. Holographic gratings formation in photopolymers: analysis and experimental results based on a non-local diffusion based model and rigorous couple-wave analysis. J. Opt. Soc. Am. B
**2003**, 20, 1177–1188. [Google Scholar] [CrossRef] - Moharam, M.G.; Young, L. Criteria for Bragg and Raman-Nath regimes. Appl. Opt.
**1978**, 17, 1757–1759. [Google Scholar] [CrossRef] [PubMed] - Moharam, M.G.; Gaylord, T.K.; Magnusson, R. Criteria for Raman-Nath regime diffraction by phase gratings. Opt. Commun.
**1980**, 32, 19–23. [Google Scholar] [CrossRef] - Moharam, M.G.; Gaylord, T.K.; Magnusson, R. Criteria for Bragg regime diffraction by phase gratings. Opt. Commun.
**1980**, 32, 14–18. [Google Scholar] [CrossRef] - Solymar, L.; Cooke, D.J. Volume Holography and Volume Gratings; Academic Press: London, UK, 1981. [Google Scholar]
- Solymar, L.; Jordan, M.P. Finite beams in large volume holograms microwaves. Opt. Acoust.
**1977**, 1, 89–92. [Google Scholar] [CrossRef] - Solymar, L.; Sheppard, C.J.R. A two-dimensional theory of volume holograms with electric polarization in the plane of the grating. J. Opt. Soc. Am.
**1979**, 69, 491–495. [Google Scholar] [CrossRef] - Fally, M.; Klepp, J.; Tomita, Y. An experimental study to discriminate between the validity of diffraction theories for off-Bragg replay. Appl. Phys. B
**2012**, in press. [Google Scholar] - Neipp, C.; Alvarez, M.L.; Gallego, S.; Ortuño, M.; Sheridan, J.T.; Pascual, I.; Beléndez, A. Angular responses of the first diffracted order in overmodulated diffraction grating. J. Modern Opt.
**2004**, 51, 1149–1162. [Google Scholar] [CrossRef] - Syms, R.R.A. Practical Volume Holography; Clarendon Press: Oxford, UK, 1990. [Google Scholar]
- Moharam, M.G.; Gaylord, T.K. Rigorous coupled-wave analysis of gratings diffraction TE-mode polarization and losses. J. Opt. Soc. Am.
**1983**, 73, 451–455. [Google Scholar] [CrossRef] - Kamiya, N. Rigorous coupled-wave analysis for practical planar dielectric gratings: 1. Thickness-changed holograms and some characteristics of diffraction efficiency. Appl. Opt.
**1998**, 37, 5843–5853. [Google Scholar] [CrossRef] [PubMed] - Moharam, M.G.; Grann, E.B.; Pommet, D.A.; Gaylord, T.K. Formulation for stable and efficient implementation of the rigorous coupled-wave analysis of binary gratings. J. Opt. Soc. Am. A
**1995**, 12, 1068–1076. [Google Scholar] [CrossRef] - Neipp, C.; Gallego, S.; Ortuño, M.; Márquez, A.; Beléndez, A.; Pascual, I. Characterization of a PVA/acrylamide photopolymer. Influence of a cross-linking monomer in the final characteristics of the hologram. Opt. Commun.
**2003**, 224, 27–34. [Google Scholar] [CrossRef] - Gallego, S.; Neipp, C.; Ortuño, M.; Beléndez, A.; Pascual, I. Stabilization of volume gratings recorded in PVA/acrylamide photopolymers with diffraction efficiencies higher than 90%. J. Modern Opt.
**2004**, 51, 491–503. [Google Scholar] [CrossRef]

© 2012 by the authors; licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution license (http://creativecommons.org/licenses/by/3.0/).

## Share and Cite

**MDPI and ACS Style**

Gallego, S.; Neipp, C.; Estepa, L.A.; Ortuño, M.; Márquez, A.; Francés, J.; Pascual, I.; Beléndez, A.
Volume Holograms in Photopolymers: Comparison between Analytical and Rigorous Theories. *Materials* **2012**, *5*, 1373-1388.
https://doi.org/10.3390/ma5081373

**AMA Style**

Gallego S, Neipp C, Estepa LA, Ortuño M, Márquez A, Francés J, Pascual I, Beléndez A.
Volume Holograms in Photopolymers: Comparison between Analytical and Rigorous Theories. *Materials*. 2012; 5(8):1373-1388.
https://doi.org/10.3390/ma5081373

**Chicago/Turabian Style**

Gallego, Sergi, Cristian Neipp, Luis A. Estepa, Manuel Ortuño, Andrés Márquez, Jorge Francés, Inmaculada Pascual, and Augusto Beléndez.
2012. "Volume Holograms in Photopolymers: Comparison between Analytical and Rigorous Theories" *Materials* 5, no. 8: 1373-1388.
https://doi.org/10.3390/ma5081373